##### In all FE simulations we run, we always have to specify the bulk modulus (or Poisson’s ratio) of all material models. In this article I will try to answer the questions: Is it important to know the bulk modulus? And does the value we specify for the bulk modulus make a big difference?

##### I will investigate this in a 3 different ways.

## 1. Uniaxial Tension of a Thermoplastic Material

We cannot easily change the bulk modulus of real materials, so it is easiest to perform our investigations using “virtual materials”. That is, I will use an accurate viscoplastic material model for thermoplastic material, here I will use the PolyUMod Three Network (TN) model, and examine the response in uniaxial tension when I change the value of the bulk modulus. The following figure shows the results from MCalibration, which is a perfect tool for this type of investigation. The figure shows that when I change the bulk modulus from 500 MPa all the way to 2000 MPa, there is virtually no change in the stress-strain response.

## 2. Uniaxial Tension of a Rubber

For completeness, I will repeat this test using a non-linear viscoelastic material model suitable for rubbers (the Bergstrom-Boyce model). In this case I varied the bulk modulus between 100 MPa and 2000 MPa. These values correspond to Poisson’s ratios between 0.48 and 0.499. The figure below shows that the stress-strain response is not changing in any significant way for this range of bulk modulus values.

## 3. Compression of an O-ring

The first 2 case studies showed that the bulk modulus does not significantly influence the stress-strain behavior in uniaxial tension. But what happens in a more realistic multiaxial test case? Here I will investigate the behavior of an o-ring that is compressed in a groove with a gap. I created a simple axisymmetric FE model using Abaqus. The mesh and boundary conditions are shown below. I simply applied a pressure on the bottom half of the o-ring in order to compress it. This may not be the most accurate method, but it is sufficient for our case study. I then assign the Bergstrom-Boyce material model to the o-ring.

The two figures below show contours of the min principal true strain for a case with a bulk modulus of 400 MPa, and a case with a bulk modulus of 2000 MPa. The figure also summarizes the max tensile strains and the max Mises stress for the two cases. It is quite interesting to see that both FE simulations give essentially identical results for the two bulk modulus values. Apparently the bulk modulus does not strongly influence the response even in this highly confined geometry.

## How to Experimentally Measure the Bulk Modulus

I recommend the following methods if you need to experimentally measure the bulk modulus of a polymer.

**Digital Image Correlation (DIC) of a tension test**

In this case you measure both the axial and transverse strains, which will allow you to determine the Poisson’s ratio, from which you can determine the bulk modulus. This works, but sometimes gives inaccurate results due to DIC noise.**Pressure – Volume – Temperature (PVT) testing**

There are specialized test equipment that allow you to mesure the specific volume as a function of pressure, from which you can calculate the bulk modulus.**Confined Compression Testing**

In this method you compress a cylindrical specimen in a hollow cylinder while you measure the pressure as a function of applied volume. This test is described in more detail in Section 2.2.9 of my “Mechanics of Solid Polymers” book.

## Summary

- You always have to specify the bulk modulus in a FE simulation
- In most FE simulations a simple guess of the bulk modulus is sufficient
- If needed, there are experimental methods that can determine the bulk modulus